**ScienceDirect**

Available online at Available online at www.sciencedirect.comwww.sciencedirect.com

## ScienceDirect

Structural Integrity Procedia 00 (2016) 000–000www.elsevier.com/locate/procedia

2452-3216 © 2016 The Authors. Published by Elsevier B.V.

Peer-review under responsibility of the Scientific Committee of PCF 2016.

### XV Portuguese Conference on Fracture, PCF 2016, 10-12 February 2016, Paço de Arcos, Portugal

## Thermo-mechanical modeling of a high pressure turbine blade of an

## airplane gas turbine engine

### P. Brandão

a_{, V. Infante}

b_{, A.M. Deus}

c_{* }

*a _{Department of Mechanical Engineering, Instituto Superior Técnico, Universidade de Lisboa, Av. Rovisco Pais, 1, 1049-001 Lisboa, }*

*Portugal *

*b _{IDMEC, Department of Mechanical Engineering, Instituto Superior Técnico, Universidade de Lisboa, Av. Rovisco Pais, 1, 1049-001 Lisboa, }*

*Portugal *

*c _{CeFEMA, Department of Mechanical Engineering, Instituto Superior Técnico, Universidade de Lisboa, Av. Rovisco Pais, 1, 1049-001 Lisboa, }*

*Portugal *

**Abstract **

During their operation, modern aircraft engine components are subjected to increasingly demanding operating conditions, especially the high pressure turbine (HPT) blades. Such conditions cause these parts to undergo different types of time-dependent degradation, one of which is creep. A model using the finite element method (FEM) was developed, in order to be able to predict the creep behaviour of HPT blades. Flight data records (FDR) for a specific aircraft, provided by a commercial aviation company, were used to obtain thermal and mechanical data for three different flight cycles. In order to create the 3D model needed for the FEM analysis, a HPT blade scrap was scanned, and its chemical composition and material properties were obtained. The data that was gathered was fed into the FEM model and different simulations were run, first with a simplified 3D rectangular block shape, in order to better establish the model, and then with the real 3D mesh obtained from the blade scrap. The overall expected behaviour in terms of displacement was observed, in particular at the trailing edge of the blade. Therefore such a model can be useful in the goal of predicting turbine blade life, given a set of FDR data.

© 2016 The Authors. Published by Elsevier B.V.

Peer-review under responsibility of the Scientific Committee of PCF 2016.

*Keywords: High Pressure Turbine Blade; Creep; Finite Element Method; 3D Model; Simulation. *

* Corresponding author. Tel.: +351 218419991.
*E-mail address: [email protected] *

Procedia Structural Integrity 7 (2017) 368–375

2452-3216 Copyright 2017 The Authors. Published by Elsevier B.V.

Peer-review under responsibility of the Scientific Committee of the 3rd International Symposium on Fatigue Design and Material Defects. 10.1016/j.prostr.2017.11.101

10.1016/j.prostr.2017.11.101 2452-3216

Copyright © 2017 The Authors. Published by Elsevier B.V.

Peer-review under responsibility of the Scientific Committee of the 3rd International Symposium on Fatigue Design and Material Defects.

### ScienceDirect

Structural Integrity Procedia 00 (2017) 000–000

www.elsevier.com/locate/procedia

2452-3216 © 2017 The Authors. Published by Elsevier B.V.

Peer-review under responsibility of the Scientific Committee of the 3rd International Symposium on Fatigue Design and Material Defects.

### 3rd International Symposium on Fatigue Design and Material Defects, FDMD 2017, 19-22 September 2017,

### Lecco, Italy

### Evaluation of Size Effect in Low Cycle Fatigue for Q&T rotor steel

### S.P. Zhu

a, b,_{*, S. Foletti}

b_{, S. Beretta}

b
*a _{School of Mechatronics Engineering, University of Electronic Science and Technology of China, Chengdu 611731, China }*

*b _{Department of Mechanical Engineering, Politecnico di Milano, Via La Masa 1, 20156 Milan, Italy }*

**Abstract **

This study presents a probabilistic modeling of size effect of 30NiCrMoV12 steel in a low cycle fatigue (LCF) regime. Three types of fatigue tests have been conducted on three geometrical specimens. Results indicate that nearly all of the LCF lifetime of 30NiCrMoV12 consists of the development of multiple surface short cracks, which has shown statistical aspects of their mutual interactions and coalescence. This gives rise to an approach of LCF damage based on statistical physics. A statistical Weibull’s weakest link model has been verified and a procedure for surface multiple fracture simulation is then established by including the random processes of initiation, propagation and coalescence of dispersed surface cracks. Using this procedure, the life of a component can be predicted from the criterion of critical cracks formation by coalescence of dispersed defects.

© 2017 The Authors. Published by Elsevier B.V.

Peer-review under responsibility of the Scientific Committee of the 3rd International Symposium on Fatigue Design and Material Defects.

*Keywords: size effect; low cycle fatigue; crack growth; statistics of extremes; crack coalescence *

**1. Introduction **

Fatigue and fracture tests are normally conducted on small test specimens of structural materials used for aircrafts and high-speed trains. In predicting the fatigue life of full scale components or structures, such as high high-speed train railway axles, the specimen size effect is critical when utilizing the laboratory testing of small standard specimens as the reference basis. In other words, fatigue testing on large specimens for those structures is not always possible due to financial considerations. Therefore, characterizing the effect of specimen size on fatigue life is needed and corresponding methods are lacking, especially a robust probabilistic method for quantifying the effect of specimen size on fatigue life.

According to the German FKM guideline launched for the strength assessment of structures under different loading conditions, the treatment of size effect is purely empirical, which is determined from empirical design curves or formulae [1-3]. The application of this size effect to other cross-sectional shapes and stress distributions is often not explained as well as the robustness of the low cycle fatigue (LCF) resistance against specimen size [4]. One of the commonly-used way to characterize the size effect by means of the weakest-link theory and the statistics of extremes. Therefore, to explain the specimen size effect toward increasing reliability of fatigue critical components, metallurgical and mechanical details must be considered in fatigue modelling and lifing procedure. Note from [5, 6] that LCF life of ductile steels is generally dominated by crack propagation life rather than crack initiation life. Namely, the effect of specimen size on the fatigue propagation rate, particularly on the scatter in small fatigue crack growth, has been viewed as the main factor influencing the fatigue life. The challenge will be to use not only the governing factors, such as

** Corresponding author. E-mail address: [email protected] *

### ScienceDirect

Structural Integrity Procedia 00 (2017) 000–000

www.elsevier.com/locate/procedia

2452-3216 © 2017 The Authors. Published by Elsevier B.V.

### 3rd International Symposium on Fatigue Design and Material Defects, FDMD 2017, 19-22 September 2017,

### Lecco, Italy

### Evaluation of Size Effect in Low Cycle Fatigue for Q&T rotor steel

### S.P. Zhu

a, b,_{*, S. Foletti}

b_{, S. Beretta}

b
*a _{School of Mechatronics Engineering, University of Electronic Science and Technology of China, Chengdu 611731, China }*

*b _{Department of Mechanical Engineering, Politecnico di Milano, Via La Masa 1, 20156 Milan, Italy }*

**Abstract **

This study presents a probabilistic modeling of size effect of 30NiCrMoV12 steel in a low cycle fatigue (LCF) regime. Three types of fatigue tests have been conducted on three geometrical specimens. Results indicate that nearly all of the LCF lifetime of 30NiCrMoV12 consists of the development of multiple surface short cracks, which has shown statistical aspects of their mutual interactions and coalescence. This gives rise to an approach of LCF damage based on statistical physics. A statistical Weibull’s weakest link model has been verified and a procedure for surface multiple fracture simulation is then established by including the random processes of initiation, propagation and coalescence of dispersed surface cracks. Using this procedure, the life of a component can be predicted from the criterion of critical cracks formation by coalescence of dispersed defects.

© 2017 The Authors. Published by Elsevier B.V.

*Keywords: size effect; low cycle fatigue; crack growth; statistics of extremes; crack coalescence *

**1. Introduction **

Fatigue and fracture tests are normally conducted on small test specimens of structural materials used for aircrafts and high-speed trains. In predicting the fatigue life of full scale components or structures, such as high high-speed train railway axles, the specimen size effect is critical when utilizing the laboratory testing of small standard specimens as the reference basis. In other words, fatigue testing on large specimens for those structures is not always possible due to financial considerations. Therefore, characterizing the effect of specimen size on fatigue life is needed and corresponding methods are lacking, especially a robust probabilistic method for quantifying the effect of specimen size on fatigue life.

According to the German FKM guideline launched for the strength assessment of structures under different loading conditions, the treatment of size effect is purely empirical, which is determined from empirical design curves or formulae [1-3]. The application of this size effect to other cross-sectional shapes and stress distributions is often not explained as well as the robustness of the low cycle fatigue (LCF) resistance against specimen size [4]. One of the commonly-used way to characterize the size effect by means of the weakest-link theory and the statistics of extremes. Therefore, to explain the specimen size effect toward increasing reliability of fatigue critical components, metallurgical and mechanical details must be considered in fatigue modelling and lifing procedure. Note from [5, 6] that LCF life of ductile steels is generally dominated by crack propagation life rather than crack initiation life. Namely, the effect of specimen size on the fatigue propagation rate, particularly on the scatter in small fatigue crack growth, has been viewed as the main factor influencing the fatigue life. The challenge will be to use not only the governing factors, such as

*S.P. Zhu et al. / Procedia Structural Integrity 7 (2017) 368–375 * 369

*2 * *S.P. Zu et al. / Structural Integrity Procedia 00 (2017) 000–000 *

local microstructure, local stress/strain, and damage physics, but also statistical approaches to understand the size effect in a LCF regime. According to this, this paper attempts to quantify the specimen size effect on fatigue lives of 30NiCrMoV12 steel from the viewpoint of mechanical-probabilistic modelling and numerical simulation of fatigue crack growth. In this paper, an alternative procedure for practical fatigue design by considering size effect will be critically investigated.

**2. Experimental **
*2.1. Material *

Low cycle fatigue tests have been conducted on specimens with three different geometries of similar shape, which are designed according to ASTM standard E606 [7] and prepared by electro-chemical polishing [8]. Figure 1 shows one of the specimen geometries used for the LCF tests. Three different specimen geometries have been manufactured to study statistical size effects. The diameter (𝐷𝐷𝐷𝐷0) and the gauge length (𝐿𝐿𝐿𝐿0) of the specimen are listed in Table 1. The specimens were made of 30NiCrMoV12

steel, which is commonly used for railway axles due to high mechanical properties and high performance. Its heat treatment includes normalization at 900℃ for uniforming and grain size refinement, then a quench treatment at 850℃ and cooling in oil bath, finally a tempering process taking at 625℃ for 12 hours in order to increase toughness. Monotonic mechanical properties of 30NiCrMoV12 are reported in Table 2.

Figure 1. Standard specimen geometry for LCF tests

Table 1. Three specimen geometries Geometry 𝐷𝐷𝐷𝐷0/𝑚𝑚𝑚𝑚𝑚𝑚𝑚𝑚 𝐿𝐿𝐿𝐿0/𝑚𝑚𝑚𝑚𝑚𝑚𝑚𝑚

G1: Standard 8 20

G2: Small 3 8

G3: Large 14 36

Table 2. Mechanical properties of 30NiCrMoV12 Elastic modulus 𝐸𝐸𝐸𝐸 197𝐺𝐺𝐺𝐺𝐺𝐺𝐺𝐺𝐺𝐺𝐺𝐺 Yield stress 𝜎𝜎𝜎𝜎𝑦𝑦𝑦𝑦 878𝑀𝑀𝑀𝑀𝐺𝐺𝐺𝐺𝐺𝐺𝐺𝐺

Ultimate tensile strength 𝜎𝜎𝜎𝜎𝑈𝑈𝑈𝑈𝑈𝑈𝑈𝑈𝑈𝑈𝑈𝑈 1045𝑀𝑀𝑀𝑀𝐺𝐺𝐺𝐺𝐺𝐺𝐺𝐺

Elongation at fracture 21.6%

*2.2. Testing *

For the investigation of LCF lifetime behaviour, MTS fatigue testing machines with maximum loads of 100 kN and 250 kN have been used for tension-compression testing. The strain range was controlled by three extensometers. All LCF tests were carried out at strain amplitude levels between 0.35% and 0.8% at load ratio 𝑅𝑅𝑅𝑅 = −1. Fatigue lifetime of the specimen is defined according to the load drop criterion. In this analysis, three types of LCF tests were performed, including typical LCF tests and replica tests on smooth/notched specimens. The latter were conducted to observe the crack length for crack growth/evolution modelling on the specimen surface, particularly, some tension-compression tests were interrupted at ﬁxed cycles and plastic replicas of the specimen surfaces were made. The quantitative crack length and numbers were determined by optical microscopy. All replica tests were performed on smooth and notched standard specimens at strain amplitude 𝜀𝜀𝜀𝜀𝑎𝑎𝑎𝑎= 0.5%. For the notched standard specimen, two

micro holes of 100𝜇𝜇𝜇𝜇𝑚𝑚𝑚𝑚 diameter were drilled with an angular distance of 120° and 1.5 millimeter far from the centre line of the
specimen. Replicas were taken during three tests on the standard specimens, three tests on the big specimen and six interrupted
tests for the small specimens. In this study, the surface cracks with length longer than 20𝜇𝜇𝜇𝜇𝑚𝑚𝑚𝑚 were measured for statistical analysis.
*2.3. Results *

In LCF analysis, a so-called strain-life approach, like the Coffin-Manson (CM) equation, is often used to describe the relationship between strain and the number of cycles to failure under uniaxial loadings, which relates the local elastic-plastic behaviour by

∆𝜀𝜀𝜀𝜀𝑡𝑡𝑡𝑡
2 =
∆𝜀𝜀𝜀𝜀𝑒𝑒𝑒𝑒
2 +
∆𝜀𝜀𝜀𝜀𝑝𝑝𝑝𝑝
2 =
𝜎𝜎𝜎𝜎𝑓𝑓𝑓𝑓′
𝐸𝐸𝐸𝐸�2𝑁𝑁𝑁𝑁𝑓𝑓𝑓𝑓�
𝑏𝑏𝑏𝑏
+ 𝜀𝜀𝜀𝜀𝑓𝑓𝑓𝑓′�2𝑁𝑁𝑁𝑁𝑓𝑓𝑓𝑓�𝑐𝑐𝑐𝑐* (1) *

where ∆𝜀𝜀𝜀𝜀𝑡𝑡𝑡𝑡, ∆𝜀𝜀𝜀𝜀𝑒𝑒𝑒𝑒 and ∆𝜀𝜀𝜀𝜀𝑝𝑝𝑝𝑝 are the total strain range, elastic strain range and plastic strain range, respectively; 𝜎𝜎𝜎𝜎𝑓𝑓𝑓𝑓′ is the fatigue strength

coefficient; 𝐸𝐸𝐸𝐸 is the Young’s modulus; 𝑁𝑁𝑁𝑁𝑓𝑓𝑓𝑓 is the number of cycles to failure; 𝑏𝑏𝑏𝑏 is the fatigue strength exponent; 𝜀𝜀𝜀𝜀𝑓𝑓𝑓𝑓′ is the fatigue

ductility coefficient; 𝑐𝑐𝑐𝑐 is the fatigue ductility exponent.

When using Eq. (1) for LCF analysis, the Ramberg-Osgood (RO) equation described the stress-strain behaviour of the material

∆𝜀𝜀𝜀𝜀𝑡𝑡𝑡𝑡
2 =
∆𝜀𝜀𝜀𝜀𝑒𝑒𝑒𝑒
2 +
∆𝜀𝜀𝜀𝜀𝑝𝑝𝑝𝑝
2 =
∆𝜎𝜎𝜎𝜎
2𝐸𝐸𝐸𝐸+ �
∆𝜎𝜎𝜎𝜎
2𝐾𝐾𝐾𝐾′�
1
𝑛𝑛𝑛𝑛′_{ }_{ (2) }

where ∆𝜎𝜎𝜎𝜎 is the tress range; 𝐾𝐾𝐾𝐾′_{ and 𝑛𝑛𝑛𝑛}′_{ are the cyclic strength coefficient and cyclic strain hardening exponent, respectively. }

Using Eq. (1) and Eq. (2), cyclic response and fatigue behaviour of three specimen sizes can be plotted as shown in Figure 2.

𝑳𝑳𝟎𝟎

*S.P. Zu et al. / Structural Integrity Procedia 00 (2017) 000–000 * * 3 *

(a) (b)

Figure 2. LCF tests of three different specimens of 30NiCrMoV12

**3. Size effect in LCF based on weakest-link modeling **
*3.1. Weakest-link theory *

The weakest link theory was originally developed by Weibull to describe the tensile fracture of brittle materials, which is based on the Weibull probability distribution of failure. Specifically, due to the randomly distributed material defects (non-homogeneities, inclusions, precipitates) in a material per volume unit, the theory states that fatigue crack initiates where the most dangerous defect or the weakest link exists [4, 9, 10]. Thus, a stochastic distribution of defects within specimens/components leads to scatter in the fatigue behaviour of the material. Through relating the effect of load and cross-sectional area with the fatigue life, a classic form of the Weibull distribution for the failure probability can be expressed as

𝐺𝐺𝐺𝐺𝑓𝑓𝑓𝑓(𝜎𝜎𝜎𝜎, 𝛺𝛺𝛺𝛺) = 1 − 𝑒𝑒𝑒𝑒𝑒𝑒𝑒𝑒𝑒𝑒𝑒𝑒 �−_{𝛺𝛺𝛺𝛺}1_{0}∫ 𝑓𝑓𝑓𝑓(𝜎𝜎𝜎𝜎)𝑑𝑑𝑑𝑑𝛺𝛺𝛺𝛺_{𝛺𝛺𝛺𝛺} *� (3) *

where 𝛺𝛺𝛺𝛺0 is the reference volume or surface; 𝑓𝑓𝑓𝑓(𝜎𝜎𝜎𝜎) is a function of the risk of rupture with three parameters

𝑓𝑓𝑓𝑓(𝜎𝜎𝜎𝜎) = �𝜎𝜎𝜎𝜎−𝜎𝜎𝜎𝜎𝑢𝑢𝑢𝑢

𝜎𝜎𝜎𝜎0 �

𝑚𝑚𝑚𝑚

* (4) *
where 𝑚𝑚𝑚𝑚 and 𝜎𝜎𝜎𝜎0 are the shape parameter and scale parameter of the Weibull distribution, respectively; 𝜎𝜎𝜎𝜎𝑢𝑢𝑢𝑢 is the threshold stress.

By using Eq. (3) for describing the life (as done by Wormsen et al. [10]), the distribution of experimental results can be derived
for specimens with diﬀerent geometries. By increasing the component volume or surface, the probability of failure increases due
to the higher probability of finding a critical defect. Thus, a relation can be obtained for two different specimen sizes under a similar
failure probability
𝑁𝑁𝑁𝑁2
𝑁𝑁𝑁𝑁1= �
𝐴𝐴𝐴𝐴1
𝐴𝐴𝐴𝐴2�
1
𝑚𝑚𝑚𝑚_{ (5) }

where 𝑁𝑁𝑁𝑁1 is the fatigue life for a specimen with the known surface or cross-sectional area 𝐴𝐴𝐴𝐴1, 𝑁𝑁𝑁𝑁2 is the estimated fatigue life for

the specimen with determined surface or cross-sectional area 𝐴𝐴𝐴𝐴2. In the current research, 𝐴𝐴𝐴𝐴1 and 𝐴𝐴𝐴𝐴2 can be calculated over the gage

section of different specimens.

Adopting Eq. (5) and taking the distribution of fatigue life of small specimens as a reference, the distribution of the life for large and standard specimens can be expressed by a function of the probability of failure of small specimens 𝐺𝐺𝐺𝐺𝑓𝑓𝑓𝑓,𝑠𝑠𝑠𝑠𝑚𝑚𝑚𝑚𝑚𝑚𝑚𝑚𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑠 as

𝐺𝐺𝐺𝐺𝑓𝑓𝑓𝑓,𝑠𝑠𝑠𝑠𝑡𝑡𝑡𝑡𝑚𝑚𝑚𝑚𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑚𝑚𝑚𝑚𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑠= 1 − �1 − 𝐺𝐺𝐺𝐺𝑓𝑓𝑓𝑓,𝑠𝑠𝑠𝑠𝑚𝑚𝑚𝑚𝑚𝑚𝑚𝑚𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑠�𝜂𝜂𝜂𝜂𝑠𝑠𝑠𝑠𝑡𝑡𝑡𝑡𝑠𝑠𝑠𝑠𝑛𝑛𝑛𝑛𝑑𝑑𝑑𝑑𝑠𝑠𝑠𝑠𝑎𝑎𝑎𝑎𝑑𝑑𝑑𝑑* (6) *

𝐺𝐺𝐺𝐺𝑓𝑓𝑓𝑓,𝑠𝑠𝑠𝑠𝑚𝑚𝑚𝑚𝑠𝑠𝑠𝑠𝑙𝑙𝑙𝑙𝑒𝑒𝑒𝑒= 1 − �1 − 𝐺𝐺𝐺𝐺𝑓𝑓𝑓𝑓,𝑠𝑠𝑠𝑠𝑚𝑚𝑚𝑚𝑚𝑚𝑚𝑚𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑠�𝜂𝜂𝜂𝜂𝑙𝑙𝑙𝑙𝑠𝑠𝑠𝑠𝑎𝑎𝑎𝑎𝑙𝑙𝑙𝑙𝑒𝑒𝑒𝑒* (7) *

where 𝜂𝜂𝜂𝜂𝑠𝑠𝑠𝑠𝑡𝑡𝑡𝑡𝑚𝑚𝑚𝑚𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑚𝑚𝑚𝑚𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑠 and 𝜂𝜂𝜂𝜂𝑠𝑠𝑠𝑠𝑚𝑚𝑚𝑚𝑠𝑠𝑠𝑠𝑙𝑙𝑙𝑙𝑒𝑒𝑒𝑒 are the ratio between gauge surfaces of the standard/large specimens and the small ones, respectively.

Under a log-normal life distribution of different sizes of specimens, Figure 3 plots life distributions of the standard and large specimens according to Eq. (6) and Eq. (7). Comparing with experimental mean and scatter of the life cycles at 𝜖𝜖𝜖𝜖𝑚𝑚𝑚𝑚= 0.5%, a

consequence of the defects distribution based on statistic of extremes cannot explain well the tested life distributions in Figure 3.

103 _{10}4 _{10}5
2N
f [cycle]
10-3
10-2
Total strain [mm/mm]

Coffin-Manson curve (standard) Coffin-Manson curve (small) Standard spec (Ø8mm) Small spec (Ø3mm) Big spec (Ø14mm) 0 0.002 0.004 0.006 0.008 0.01 0.012 0.014 Total strain [mm/mm] 0 100 200 300 400 500 600 700 s [Mpa]

Ramberg-Osgood curve (standard) Ramberg-Osgood curve (small) Standard spec (Ø8mm) Small spec (Ø3mm) Big spec (Ø14mm)

*S.P. Zhu et al. / Procedia Structural Integrity 7 (2017) 368–375 * 371

*4 * *S.P. Zu et al. / Structural Integrity Procedia 00 (2017) 000–000 *

Figure 3. Expected life based only on size effect due to statistic of extremes
*3.2. Fatigue crack growth life *

Note from Figure 4 that the inspection of fracture surfaces with SEM show that most cracks initiated at the surface of the specimen. For 30NiCrMoV12 steel, its LCF life is obviously dominated by crack propagation life rather than crack initiation life. Thus, the effect of specimen geometrical size on the fatigue crack propagation rate is critical essential for a theoretical understanding of fatigue lives.

(a) (b) (c)

Figure 4. Multiple surface cracks of (a) small, (b) standard and (c) large specimen

Fatigue crack growth in the presence of a marked plastic strain range under LCF conditions can be well described by using Tomkins model [11]. Through assuming the amount of crack growth per cycle under tension-compression loadings to be the amount of irreversible shear decohesion which occurs at the crack tip, Tomkins [11] correlates crack growth to the plastic strain amplitude in an exponential law

�_{𝑘𝑘𝑘𝑘}𝐺𝐺𝐺𝐺 = 𝐺𝐺𝐺𝐺𝑖𝑖𝑖𝑖𝑒𝑒𝑒𝑒𝑘𝑘𝑘𝑘𝑙𝑙𝑙𝑙𝑁𝑁𝑁𝑁

𝑙𝑙𝑙𝑙= 𝑘𝑘𝑘𝑘𝑙𝑙𝑙𝑙0𝜀𝜀𝜀𝜀𝑝𝑝𝑝𝑝𝑎𝑎𝑎𝑎𝑠𝑠𝑠𝑠 * (8) *

where 𝐺𝐺𝐺𝐺 and 𝐺𝐺𝐺𝐺𝑖𝑖𝑖𝑖 are the crack length and initial crack length, respectively; 𝜀𝜀𝜀𝜀𝑝𝑝𝑝𝑝𝑎𝑎𝑎𝑎 is the plastic strain amplitude, 𝑘𝑘𝑘𝑘𝑙𝑙𝑙𝑙0 and 𝑑𝑑𝑑𝑑 are material

parameters that establish the short cracks growth in a material. Accordingly, a simplified form can be expressed as

𝑠𝑠𝑠𝑠𝑎𝑎𝑎𝑎

𝑠𝑠𝑠𝑠𝑁𝑁𝑁𝑁= 𝑘𝑘𝑘𝑘𝑙𝑙𝑙𝑙*𝐺𝐺𝐺𝐺 (9) *

The number of cycles is obtained by integrating Eq. (9) from an initial crack length 𝐺𝐺𝐺𝐺𝑖𝑖𝑖𝑖 to a final one 𝐺𝐺𝐺𝐺𝑓𝑓𝑓𝑓. Parameter of Eq. (9)

was calibrated from experiments, as shown in Figure 5. Two scale factors can be obtained to shift the distribution found with the statics of extremes for the standard/large specimen from the reference small one

𝛾𝛾𝛾𝛾𝑠𝑠𝑠𝑠𝑡𝑡𝑡𝑡𝑎𝑎𝑎𝑎𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑎𝑎𝑎𝑎𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑠=∆𝑁𝑁𝑁𝑁_{∆𝑁𝑁𝑁𝑁}𝑠𝑠𝑠𝑠𝑡𝑡𝑡𝑡𝑠𝑠𝑠𝑠𝑛𝑛𝑛𝑛𝑛𝑛𝑛𝑛𝑠𝑠𝑠𝑠𝑎𝑎𝑎𝑎𝑛𝑛𝑛𝑛_{𝑠𝑠𝑠𝑠𝑚𝑚𝑚𝑚𝑠𝑠𝑠𝑠𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙} =
𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑠�𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙10�𝑠𝑠𝑠𝑠𝑓𝑓𝑓𝑓,𝑠𝑠𝑠𝑠𝑡𝑡𝑡𝑡𝑠𝑠𝑠𝑠𝑛𝑛𝑛𝑛𝑛𝑛𝑛𝑛𝑠𝑠𝑠𝑠𝑎𝑎𝑎𝑎𝑛𝑛𝑛𝑛�
𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙10�𝑠𝑠𝑠𝑠𝑖𝑖𝑖𝑖� �
𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑠�𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙10�𝑠𝑠𝑠𝑠𝑓𝑓𝑓𝑓,𝑠𝑠𝑠𝑠𝑚𝑚𝑚𝑚𝑠𝑠𝑠𝑠𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙�_{𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙10�𝑠𝑠𝑠𝑠𝑖𝑖𝑖𝑖�} �
* (10) *
𝛾𝛾𝛾𝛾𝑠𝑠𝑠𝑠𝑎𝑎𝑎𝑎𝑠𝑠𝑠𝑠𝑙𝑙𝑙𝑙𝑒𝑒𝑒𝑒=∆𝑁𝑁𝑁𝑁_{∆𝑁𝑁𝑁𝑁}𝑙𝑙𝑙𝑙𝑠𝑠𝑠𝑠𝑎𝑎𝑎𝑎𝑙𝑙𝑙𝑙𝑒𝑒𝑒𝑒_{𝑠𝑠𝑠𝑠𝑚𝑚𝑚𝑚𝑠𝑠𝑠𝑠𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙}=
𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑠�𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙10�𝑠𝑠𝑠𝑠𝑓𝑓𝑓𝑓,𝑙𝑙𝑙𝑙𝑠𝑠𝑠𝑠𝑎𝑎𝑎𝑎𝑙𝑙𝑙𝑙𝑒𝑒𝑒𝑒�
𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙10�𝑠𝑠𝑠𝑠𝑖𝑖𝑖𝑖� �
𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑠�𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙10�𝑠𝑠𝑠𝑠𝑓𝑓𝑓𝑓,𝑠𝑠𝑠𝑠𝑚𝑚𝑚𝑚𝑠𝑠𝑠𝑠𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙�
𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙10�𝑠𝑠𝑠𝑠𝑖𝑖𝑖𝑖� �
* (11) *
Combining Eq. (6) to Eq. (11), the life scale factors at 𝜖𝜖𝜖𝜖𝑎𝑎𝑎𝑎= 0.5% due to the propagation size effect can be calculated from an

initial crack length 𝐺𝐺𝐺𝐺𝑖𝑖𝑖𝑖= 100𝜇𝜇𝜇𝜇𝑚𝑚𝑚𝑚 to a final crack length 𝐺𝐺𝐺𝐺𝑓𝑓𝑓𝑓=𝜋𝜋𝜋𝜋𝐷𝐷𝐷𝐷_{2}0, namely, 𝛾𝛾𝛾𝛾𝑠𝑠𝑠𝑠𝑡𝑡𝑡𝑡𝑎𝑎𝑎𝑎𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑎𝑎𝑎𝑎𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑠= 1.18048 and 𝛾𝛾𝛾𝛾𝑠𝑠𝑠𝑠𝑎𝑎𝑎𝑎𝑠𝑠𝑠𝑠𝑙𝑙𝑙𝑙𝑒𝑒𝑒𝑒= 1.27523.

As pointed out by Koyama et al. [5], the specimen size effect can be quantified by the sum of the effect of statistical distribution

2.5 3 3.5 4 4.5 Log 10(2N) 0 0.5 1 1.5 2 2.5 3 3.5 4 4.5 PDF

**Evaluation of size effect with statistic of extremes**

Small specimen by testing Standard specimen by testing Large specimen by testing Standard specimen by Eq. (6) Large specimen by Eq. (7)

of the defects and the effect of crack propagation. From a crack growth point of view, a larger specimen would lead to a longer life,
*which shift the dotted/dash lines in Figure 3 to the right-hand of the x-axis. According to this, a comparison between the curves of *
experimental distribution of the life and the ones due to the effects of statistical defects and crack propagation can be made by using
Eq. (10) and Eq. (11), as shown in Figure 6 and results in Table 3.

Figure 5 Crack growth measurement near the micro hole

Figure 6. Comparison between extracted distribution and experimental ones

Table 3 Mean and scatter of the life cycles at 𝜖𝜖𝜖𝜖𝑎𝑎𝑎𝑎= 0.5% due to the

combination of propagation and statistical distribution of defects Experimental /

𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙10(𝐶𝐶𝐶𝐶𝐶𝐶𝐶𝐶𝑐𝑐𝑐𝑐𝑙𝑙𝑙𝑙𝑐𝑐𝑐𝑐)

Extracted / 𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙𝑙10(𝐶𝐶𝐶𝐶𝐶𝐶𝐶𝐶𝑐𝑐𝑐𝑐𝑙𝑙𝑙𝑙𝑐𝑐𝑐𝑐)

𝜇𝜇𝜇𝜇% error

Standard spec. Mean 3.6807 3.6382 _{1.15% }

Std. 0.1557 0.1759

Large spec. Mean 3.7021 3.7441 _{1.13% }

Std. 0.0779 0.1620

**4. Numerical modeling of multiple fracture **

As aforementioned, the weakest-link theory assumed that the critical defects do not interact which are sparsely distributed. This assumption only works under limited number of potentially critical defect sites. As noticed from Figure 4, the presence of multiple surface cracks scatted over the gauge section is the main manifestation of damages in 30NiCrMoV12 steel under cyclic loadings. In particular, its fracture was induced by the processes of initiation, growth and coalescence of cracks. Combining with the replica tests as mentioned in Section 2, a numerical Monte Carlo simulation is performed for multiple fracture evaluation and to compare experimental data on crack length distribution evolution, as well as their experimental lives, with the simulated ones.

*4.1. Initial prerequisites of the model *

The simulation conducted in this analysis includes the process of random crack initiation, propagation and coalescence of surface microcracks occurring simultaneously. According to available experimental data on replica tests under cyclic loadings, the initial prerequisites and assumptions are taken as follows.

(1) Uniform material properties are assumed over the entire damaged surface, namely, the simulation surface area; (2) Uniaxial stress state is loaded and time-independent during the crack evolution;

*(3) All cracks on the surface are oriented normally to the stress action direction, like the x-axis in this analysis; *
(4) A constant increment of the load cycles is assigned as the count number of iterations;

(5) The positions of all cracks on the surface are randomly distributed according to Poisson’s law. Particularly, the probability
*that n cracks are located on the area A with the crack density 𝜆𝜆𝜆𝜆 *

𝐺𝐺𝐺𝐺(𝑛𝑛𝑛𝑛) =(−𝜆𝜆𝜆𝜆𝐴𝐴𝐴𝐴)_{𝑠𝑠𝑠𝑠!} 𝑛𝑛𝑛𝑛*𝑐𝑐𝑐𝑐𝑒𝑒𝑒𝑒𝑒𝑒𝑒𝑒(−𝜆𝜆𝜆𝜆𝐴𝐴𝐴𝐴) (12) *
(6) The initial length 𝐺𝐺𝐺𝐺 of the crack is assigned by a two-parameter Weibull distribution;

𝐺𝐺𝐺𝐺(𝐺𝐺𝐺𝐺) = 1 − 𝑐𝑐𝑐𝑐𝑒𝑒𝑒𝑒𝑒𝑒𝑒𝑒 �− �𝑎𝑎𝑎𝑎−𝑎𝑎𝑎𝑎0

𝛼𝛼𝛼𝛼 �

𝛽𝛽𝛽𝛽

*� (13) *
where 𝛽𝛽𝛽𝛽 and 𝛼𝛼𝛼𝛼 are the Weibull shape parameter and scale parameter, which were obtained from measurements on the plastic
replicas, and 𝐺𝐺𝐺𝐺0 is the resolution of crack identification.

(7) In crack propagation, the crack length increment for any crack within a given number of iterations is prescribed;

(8) In crack coalescence, quasi-collinear cracks in close proximity interact through the influence zones at both tips, which shows the changes in their propagation paths when their tips approach one another [12]. The influence zone is defined by a circle of diameter 𝑟𝑟𝑟𝑟𝑝𝑝𝑝𝑝 according to the size of local plastic deformation zone at the crack tip [13]

𝟏𝟏𝟏𝟏𝟏𝟏𝟏𝟏 𝒄𝒄𝒄𝒄𝒄𝒄𝒄𝒄𝒄𝒄𝒄𝒄 𝟏𝟏𝟏𝟏𝟏𝟏𝟏𝟏 𝒄𝒄𝒄𝒄𝒄𝒄𝒄𝒄𝒄𝒄𝒄𝒄 𝟐𝟐𝟐𝟐𝟏𝟏𝟏𝟏 𝒄𝒄𝒄𝒄𝒄𝒄𝒄𝒄𝒄𝒄𝒄𝒄
2.5 3 3.5 4 4.5
Log_{10}(2N)
0
0.5
1
1.5
2
2.5
3
3.5
4
4.5
PDF

**Comparison between experimental data end the sum of the size effects**

Small specimen experimental Standard specimen experimental Large specimen experimental Standard specimen superposition Large specimen superposition

*S.P. Zhu et al. / Procedia Structural Integrity 7 (2017) 368–375 * 373

*6 * *S.P. Zu et al. / Structural Integrity Procedia 00 (2017) 000–000 *

𝑟𝑟𝑟𝑟𝑝𝑝𝑝𝑝=𝛥𝛥𝛥𝛥𝐽𝐽𝐽𝐽𝑒𝑒𝑒𝑒𝑓𝑓𝑓𝑓𝑓𝑓𝑓𝑓∙𝐸𝐸𝐸𝐸

′

2𝜋𝜋𝜋𝜋𝜎𝜎𝜎𝜎02 * (14) *

where ∆𝐽𝐽𝐽𝐽𝑒𝑒𝑒𝑒𝑓𝑓𝑓𝑓𝑓𝑓𝑓𝑓* is the effective cyclic J-Integral, 𝜎𝜎𝜎𝜎*0 is the flow stress and 𝐸𝐸𝐸𝐸′ is the cyclic Young’s Modulus under plane strain

conditions, 𝐸𝐸𝐸𝐸′_{= 𝐸𝐸𝐸𝐸 (1 − 𝑣𝑣𝑣𝑣}_{⁄} 2_{)}_{ and 𝑣𝑣𝑣𝑣 is the Poisson’s ratio. }

The criterion of Murakami [14] on judging defects interaction/coalescence is adopted, by the distance between the tips 𝑑𝑑𝑑𝑑 is less than the minimum of the two crack length

𝑑𝑑𝑑𝑑 < 𝑚𝑚𝑚𝑚𝑚𝑚𝑚𝑚𝑛𝑛𝑛𝑛(𝐺𝐺𝐺𝐺𝑐𝑐𝑐𝑐𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑐𝑐𝑐𝑐𝑘𝑘𝑘𝑘1, 𝐺𝐺𝐺𝐺𝑐𝑐𝑐𝑐𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑠𝑐𝑐𝑐𝑐𝑘𝑘𝑘𝑘2) (15)

(9) An unloaded material zone during crack propagation and coalescence is formed around each crack, of which the shape of the zone is defined as a circle of diameter equal to the crack length. In these zones, the crack growth is arrested if its tip comes into the unloading zone from the nearest crack.

Based on abovementioned starting prerequisites, a simulation flow chart is given in Figure 7, the basic inputs obtained from experimental testing for multiple fracture simulation of different geometrical specimens include the following parameters:

(1) Crack density on the surface; (2) Damage surface size;

(3) Distribution of crack length and crack growth rate (without regard for the crack coalescence) on the surface; (4) Fracture and failure criterion.

Figure 7. Main flow chart of multiple fracture simulation
**Input source data**

𝐶𝐶𝐶𝐶𝑟𝑟𝑟𝑟𝐺𝐺𝐺𝐺𝐶𝐶𝐶𝐶𝐶𝐶𝐶𝐶 𝑑𝑑𝑑𝑑𝑚𝑚𝑚𝑚𝑑𝑑𝑑𝑑𝑟𝑟𝑟𝑟𝑚𝑚𝑚𝑚𝑑𝑑𝑑𝑑𝑑𝑑𝑑𝑑𝑚𝑚𝑚𝑚𝑑𝑑𝑑𝑑𝑛𝑛𝑛𝑛 𝐺𝐺𝐺𝐺𝑑𝑑 2𝐸𝐸𝐸𝐸𝐸 𝐶𝐶𝐶𝐶𝑐𝑐𝑐𝑐𝐶𝐶𝐶𝐶𝑐𝑐𝑐𝑐𝑐𝑐𝑐𝑐𝑑𝑑 𝜆𝜆𝜆𝜆, 𝛼𝛼𝛼𝛼, 𝛽𝛽𝛽𝛽, 𝐴𝐴𝐴𝐴, 𝐺𝐺𝐺𝐺𝑓𝑓𝑓𝑓, 𝐶𝐶𝐶𝐶𝑙𝑙𝑙𝑙, 𝜀𝜀𝜀𝜀𝑠𝑠𝑠𝑠, 𝜎𝜎𝜎𝜎0, 𝐸𝐸𝐸𝐸

**Start**

**End**
**Random crack initiation**

Crack position: Poisson’s law

Crack length: Weibull distribution

For 𝑗𝑗 = 1 iteration

Δ𝑁𝑁𝑁𝑁/𝐶𝐶𝐶𝐶𝑐𝑐𝑐𝑐𝐶𝐶𝐶𝐶𝑐𝑐𝑐𝑐𝑐𝑐𝑐𝑐𝑑𝑑

**Crack coalescence analysis**

Unloaded and influence zone identification

Crack propagation type

Calculation of crack tip distance

Merge cracks or change crack tip angles

**Crack propagation**

Increment of crack length 𝑑𝑑𝑑𝑑𝐺𝐺𝐺𝐺

Crack growth rate: random variable vs. random process

Track the largest critical crack 𝐺𝐺𝐺𝐺𝑚𝑚𝑚𝑚𝑠𝑠𝑠𝑠𝑚𝑚,𝑗𝑗

If maximum crack length

𝐺𝐺𝐺𝐺𝑚𝑚𝑚𝑚𝑠𝑠𝑠𝑠𝑚𝑚,𝑗𝑗> 𝐺𝐺𝐺𝐺𝑓𝑓𝑓𝑓

**Calculation of life**

𝑁𝑁𝑁𝑁𝑓𝑓𝑓𝑓,𝑖𝑖𝑖𝑖= 2𝐸𝐸𝐸𝐸𝐸 + 𝑗𝑗∆𝑁𝑁𝑁𝑁

𝑗𝑗 = 𝑗𝑗 + 1

For 𝑚𝑚𝑚𝑚 = 1 to total simulation number (102_{)}

Monte Carlo sampling

**Continue?**
**Life distribution 𝑵𝑵**𝒇𝒇

No Yes

*4.2. Simulation results and discussions *

During simulation, the material damaging under cyclic loading can be characterized by crack initiation, propagation and coalescence, which are dispersed over the surface with different lengths as shown in Figure 8. Two mechanisms of crack propagation, namely, crack length increment due to its own growth for those cracks without coalescence and sudden crack length increment due to the neighbouring cracks coalescence through interacting by their tips, are involved in this simulation. Accordingly, the largest crack exhibits jump-like growth due to merging with other cracks in the plastic radius. Through following the procedure in Section 4.1, an example probability plot of experimental and simulated lives on small specimens is presented in Figure 9. Note that the simulated life distribution covers well with the lives of small specimens except that of G2.13 and G2.14, in which their fracture surfaces in Figure 10 have shown the worst condition on multiple surface crack interaction and propagation.

(a) (b)

Figure 8. Scheme of crack distribution and unloaded zones (a) Surface crack simulation at 𝜀𝜀𝜀𝜀𝑎𝑎𝑎𝑎= 0.5% (circles mark the unloaded zones, square marks the crack

coalescence) and (b) Replica on specimen G 2.12 at 3E3 cycles

(a) (b)

Figure 9. Comparison between experimental and simulated lives of small specimen: (a) probability plot and (b) life distribution

(a) G2.13 (b) G2.14 Figure 10. Fracture surface of small specimens

**5. Conclusions **

In this study, we proposed a probabilistic modelling and numerical simulation procedure for evaluating the effects of specimen size on fatigue life with three different geometrical specimens. Specifically, the specimen size effect is quantified from two categorizes, namely, size effect due to the effects of statistical defects and crack propagation, which provides a reference for fatigue

3 3.1 3.2 3.3 3.4 3.5 3.6 3.7 3.8 3.9 4
Log_{10}Cycle
-3
-2
-1
0
1
2
3
z =
1 (q)

**Log-Normal probability plot Small spec. life comparison between simulated and experimental life**

Experimental point
Fitted curve
95% confidence band
5% confidence band
Simulated point
𝑮𝑮𝑮𝑮. 𝟏𝟏𝟏𝟏
𝑮𝑮𝑮𝑮. 𝟏𝟏𝟏𝟏
3 3.1 3.2 3.3 3.4 3.5 3.6 3.7 3.8 3.9 4
Log_{10}Cycle
0
1
2
3
4
5
6
7
8
PDF

**Log-normal distributions of life comparison between small specimens **

Simulated point Experimental point Experimental distribution Simulated distribution

*S.P. Zhu et al. / Procedia Structural Integrity 7 (2017) 368–375 * 375

*8 * *S.P. Zu et al. / Structural Integrity Procedia 00 (2017) 000–000 *

life estimation under different specimen sizes. Moreover, a simulation procedure for surface multiple fracture is established by including the random processes of initiation, propagation and coalescence of dispersed surface cracks, which accounts for the observed experimental scatter in fatigue lifetime of small specimen of 30NiCrMoV12 steel. Using this procedure, the life of a component can be predicted from the criterion of critical cracks formation by coalescence of dispersed defects.

**Acknowledgments **

Dr. S.P. Zhu acknowledges support for his period of study at Politecnico di Milano by the Polimi International Fellowship Grant scheme. The authors acknowledged support by Lucchini RS (Italy) for supplying the heat treated steel.

**References **

*[1] O. Hertel, M. Vormwald, “Statistical and geometrical size effects in notched members based on weakest-link and short-crack modelling,” Eng. Fract. Mech., *
vol. 95, pp. 72–83, 2012.

*[2] M. Makkonen, “Statistical size effect in the fatigue limit of steel,” Int. J. Fatigue, vol. 23, no. 5, pp. 395–402, 2001. *

*[3] S.P. Zhu, S. Foletti, S. Beretta, “Probabilistic framework for multiaxial LCF assessment under material variability,” Int. J. Fatigue, in press, *
https://doi.org/10.1016/j.ijfatigue.2017.06.019, 2017.

[4] T. Tomaszewski, J. Sempruch, T. Piatkowski, “Verification of selected models of the size effect based on high-cycle fatigue testing on mini specimens made of
*EN AW-6063 Aluminum alloy,” J. Theor. Appl. Mech., vol. 52, no. 4, pp. 883–894, 2014. *

[5] M. Koyama, H. Li, Y. Hamano, and T. Sawaguchi, “Mechanical-probabilistic evaluation of size effect of fatigue life using data obtained from single smooth
*specimen : An example using Fe-30Mn-4Si-2Al seismic damper alloy,” Eng. Fail. Anal., vol. 72, pp. 34–47, 2017. *

*[6] Y. Murakami, K. J. Miller, “What is fatigue damage ? A view point from the observation of low cycle fatigue process,” Int. J. Fatigue, vol. 27, pp. 991–1005, *
2005.

*[7] “ASTM Standard E606. Standard Practice for Strain-Controlled Fatigue Testing,” Annu. B. ASTM Stand. 3, ASTM Int., 2004. *

*[8] T. S. Hahn, A. R. Marder, “Effect of electropolishing variables on the current density- voltage relationship,” Metallography, vol. 21, pp. 365–375, 1988. *
*[9] F. W. Zok, “On weakest link theory and Weibull statistics,” J. Am. Ceram. Soc., vol. 100, pp. 1265–1268, 2017. *

[10] A. Wormsen, B. Sjödin, G. Härkegård, and A. Fjeldstad, “Non-local stress approach for fatigue assessment based on weakest-link theory and statistics of
*extremes,” Fatigue Fract. Eng. Mater. Struct., vol. 30, no. 12, pp. 1214–1227, 2007. *

*[11] Tomkins B, “Fatigue crack propagation - an analysis,” Philos. Mag., vol. 18, no. 155, pp. 1041–1066, 1968. *

*[12] H.Y. Yoon, S.C. Lee, “Probabilistic distribution of fatigue crack growth life considering effect of crack coalescence,” JSME Int. J. Ser. A Solid Mech. Mater. *

*Eng., vol. 46, no. 4, pp. 607–612, 2003. *

[13] S. Rabbolini, S. Beretta, S. Foletti, M. E. Cristea, “Crack closure effects during low cycle fatigue propagation in line pipe steel: An analysis with digital image
*correlation,” Eng. Fract. Mech., vol. 148, pp. 441–456, 2015. *